Journal of Oral Rehabilitation 2014 41; 314--322
Enamel wear caused by monolithic zirconia crowns after 6 months of clinical use T. STOBER*, J. L. BERMEJO†, P. RAMMELSBERG* & M. SCHMITTER*
Prosthodontics, University Hospital Heidelberg, Heidelberg, and †Institute of Medical Biometry and Informatics, University Hospital Heidelberg, Heidelberg, Germany
The purpose of this study was to evaluate enamel wear caused by monolithic zirconia crowns and to compare this with enamel wear caused by contralateral natural antagonists. Twenty monolithic zirconia crowns were placed in 20 patients requiring full molar crowns. For measurement of wear, impressions of both jaws were made at baseline after crown cementation and at 6-month follow-up. Mean and maximum wear of the occlusal contact areas of the crowns, of their natural antagonists and of the two contralateral natural antagonists were measured by the use of plaster replicas and 3D laser scanning methods. Wear differences were investigated by the use of two-sided paired Student’s t-tests and by linear regression analysis. Mean vertical loss (maximum vertical loss in parentheses) was 10 (43) lm for the zirconia crowns, 33 (112) lm for the opposing enamel, 10 (58) lm for the contralateral teeth and 10 (46) lm for the contralateral SUMMARY
Introduction All-ceramic restorations have become increasingly popular in recent years, mainly because of their excellent biocompatibility and aesthetics (1). Today many different all-ceramic systems are available. They differ in their microstructure (predominantly glassy ceramics, particle-filled glasses, polycrystalline ceramics), manufacturing technique and clinical application (1, 2). The availability of computer-aided design and manufacture has enabled the construction of well-fitting frameworks for crowns and fixed partial dentures © 2014 John Wiley & Sons Ltd
antagonists. Both mean and maximum enamel wear were significantly different between the antagonists of the zirconia crowns and the contralateral antagonists. Gender and activity of the masseter muscle at night (bruxism) were identified as possible confounders which significantly affected wear. Under clinical conditions, monolithic zirconia crowns seem to be associated with more wear of opposed enamel than are natural teeth. With regard to wear behaviour, clinical application of monolithic zirconia crowns is justifiable because the amount of antagonistic enamel wear after 6 months is comparable with, or even lower than, that caused by other ceramic materials in previous studies. KEYWORDS: crowns, restoration occlusal wear, tooth wear, wear, zirconia, zirconium oxide Accepted for publication 23 December 2013
from high-strength polycrystalline ceramics, for example transformation-toughened zirconium dioxide (zirconia) (1–3). The scientific literature shows that zirconia has proved to be a suitable substructure ceramic with a wide range of indications, among others, for large fixed partial dentures in stress-bearing regions (1–9). Clinical studies have indicated that zirconia-based fixed partial dentures may be regarded as viable restorations in the anterior and posterior dentition with excellent clinical short-term survival (5, 6, 8, 9). The opaque white colour of zirconia must be doi: 10.1111/joor.12139
ENAMEL WEAR CAUSED BY MONOLITHIC ZIRCONIA CROWNS veneered with glassy ceramic, however, and fracture or chipping of the ceramic veneer has been reported to be a major complication (2, 9–13). Several proposals for overcoming the chipping problem have been published (14–16), and as a result of advances in CAD/CAM technology and the techniques used for zirconia materials, CAD/CAM fabricated nonveneered, monolithic zirconia restorations have become increasingly popular. One basic requirement for monolithic restorations was the introduction of zirconia with increased translucency; this was achieved by modifications of the fabrication process and the sintering procedures (17). Furthermore, to achieve acceptable aesthetics, pre-stained zirconia and shading liquids which match the natural tooth colour are available. It is unclear how the mechanical properties and autocatalytic surface transformation (low-temperature degradation) of zirconia are affected by these modifications. One in vitro study revealed that monolithic, full-contour zirconia crowns have higher fracture toughness than veneered zirconia-based crowns (18). The first encouraging clinical reports of monolithic zirconia crowns are now available (19). A question of special interest is the wear behaviour of monolithic zirconia restorations, in particular, wear of the enamel of natural antagonists opposed to the extremely hard zirconia material. Several in vitro studies have addressed this topic by the use of different wear simulation devices. The results of these studies indicate that zirconia has high wear resistance and, compared with other dental ceramics, causes similar or less wear of different antagonistic materials (human enamel, steatite, synthetic hydroxyapatite, stainless steel) (18, 20–27). Results relating to techniques for finishing and polishing the zirconia surface are controversial. One study reported lower wear of the antagonist material with glazed zirconia (18), whereas other studies showed that well-polished surfaces without glaze can reduce wear of opposing materials (21, 24–26). In vitro wear studies have shortcomings, however. For example, they evaluate wear behaviour by simulation of only one or two wear mechanisms under limited chewing simulation conditions. All wear methods lack evidence of clinical relevance (28). There is, therefore, a need to assess the clinical wear behaviour of zirconium dioxide restorations. © 2014 John Wiley & Sons Ltd
The objectives of this clinical study were: 1 to quantify enamel wear caused by antagonistic monolithic zirconia crowns and 2 to quantify the wear of the zirconia crowns by opposing natural dentition. Two contralateral, not crowned, antagonists with occlusal enamel contacts served as controls. The null hypothesis was that monolithic zirconia crowns and natural teeth cause comparable wear of opposing enamel under clinical conditions.
Methods Participants The Ethics Committee of the University Hospital, Heidelberg, independently reviewed and approved the study (ethical approval: local university review board, no. 222/2010). Written consent was a precondition for participation. Thirty-three patients requiring full crowns on molars were screened, and 20 were included in the study. To meet the inclusion criteria, the patients needed a natural (not crowned) opposing antagonist and two natural (not crowned) contralateral antagonistic teeth. Teeth with fillings were allowed if at least one occlusal contact point was enamel. Subjects with clinical signs of bruxism [attrition score >2 according to Wigdorowicz-Makowerowa et al. (29), muscle pain], subjects who reported grinding and/or clenching and subjects who reported other medical or mental disorders and/or sleep disorders were excluded (30, 31). Subjects meeting the inclusion criteria were examined in a second step by the use of a disposable electromyographic device (BiteStrip, up2dent). Severe muscle activity at night (more than 100 episodes within 5 h) was observed for nine subjects who were therefore excluded from the clinical trial. Four other subjects had to be excluded because thorough examination revealed missing enamel occlusal contact points of contralateral antagonists. The age of the 20 participants ranged from 21 to 73 years (mean age 43, s.d. 14); 10 participants (50%) were male. Clinical procedures and fabrication of the crowns All clinical and technical procedures were performed in strict agreement with a clinical and technical instruction protocol. Before crown preparation, lost
T . S T O B E R et al. tooth structure was replaced by core build-up with adhesively retained composite resin (Rebilda SC*). Teeth were prepared by the removal of 05–07 mm (circular) and 10–12 mm (occlusal) with a pronounced circumferential chamfer at the preparation margin. Our objective was to achieve a 4° convergence angle of the tooth preparation. Conventional impressions were obtained in polyether, by the use of a one-step, dual-viscosity technique (Impregum Penta Soft and Impregum Garant L Duosoft†), and sent to the participating laboratory where working casts of type IV gypsum (Sherahardrock‡) were subsequently made. The crowns were made of translucent, pre-shaded, yttrium-stabilised zirconia (Zenostar Zr Translucent§) by the Zenostar method, that is, fabrication of nonveneered, monolithic crowns by the following: 1 3D scanning of the working casts and working dies (D700 3D scanner¶) 2 design of the dental restoration by the technician by the use of CAD/CAM software (3shape CAD Design Software¶) and 3 transfer of the digitally adjusted data to a milling machine (Zenotec 4030 M1§) which cuts the zirconia crown to the final form. As needed, after the milling process, the crowns were thoroughly adapted and the occlusal surfaces were characterised with fine-grit diamond burs before sintering. The crowns were sintered at 1520 °C for 3 h in a high-temperature sinter furnace (Zenotec fire§). Subsequently, the crowns, particularly the occlusal surfaces, were polished with the polishing equipment recommended by the manufacturer (Zenostar Polishing Set§). After polishing, the crowns were cleaned with a steam jet and glazed with a glaze spray (Zenostar Magic Glaze Spray§). They were then stained and characterised by means of shading pastes (Zenostar Color Zr§) to match the natural tooth colour. Firing of the glaze at 850 °C for 2 min (Vitamat 2500**) completed the manufacturing process.
During the intra-oral try-ins, perfect fit, occlusion and aesthetics of the crowns were checked. Unavoidable occlusal adjustments were performed with fine-grit diamond burs; the surfaces were subsequently polished thoroughly with a set of diamond-impregnated polishers (Zenostar Polishing Set§). The crowns were luted non-adhesively to the abutment teeth by the use of glass–ionomer cement (Ketac Cem Aplicap†). Follow-ups and wear evaluations To evaluate wear, impressions were made at baseline (1–2 weeks after insertion) and after 6 months (24 2 weeks after insertion). Two impressions (one each of the maxilla and the mandible) were taken with a vinylpolysiloxane impression material (Virtual putty and Virtual light††), by the use of the dual-viscosity technique. Replicas were made of type IV dental stone (GC Fujirock EP Pearl White‡‡; GC Europe N.V., Leuven, Belgium). The occlusal contact points of the zirconia crowns, of their antagonists, and of the two contralateral antagonistic teeth (control teeth) were intra-orally marked with 12-lm Hanel occlusion foil§§. The clinical status, particularly the marked occlusal contact points were photographed to determine the occlusal contact areas (OCA) for wear measurement and the reference areas for occlusal matching. Occlusal wear was measured with a 3D laser scanner, by the method described by Mehl et al. (32). First, the occlusal surfaces of the replicas were digitised by the use of a three-dimensional optical profilometer (Laserscan 3D¶¶). The data sets obtained in this way were then checked for surface changes or wear by the use of surface analysis software (MATCH 3D, version 1.6¶¶). The extent of wear was calculated by superimposing the baseline data on those from the follow-up (occlusal matching). A matching method without reference points, as described by Mehl et al., (32) was used; this enables determination of surface changes with accuracy of 10 lm. To prevent surface changes as a result of wear or artefacts in the replicas (voids in the stone, etc.) from impairing the superim-
*Voco, Cuxhaven, Germany. †
3M Espe, Seefeld, Germany.
Shera, Lemf€ orde, Germany.
Wieland Dental, Pforzheim, Germany.
3shape, Copenhagen, Denmark.
**Vita Zahnfabrik, Bad S€ackingen, Germany.
Ivoclar Vivadent, Schaan, Liechtenstein. Leuven, Belgium. Colt ene Whaledent, Langenau, Germany.
Willytec, Gr€ afelfing, Germany. © 2014 John Wiley & Sons Ltd
ENAMEL WEAR CAUSED BY MONOLITHIC ZIRCONIA CROWNS
Fig. 1. (a–c) Example of a zirconia crown on molar 16 (Zenostar Zr Translucent; Wieland Dental) 1 week after incorporation (a) and after 6 months (b). Differential image of the replica scans showing material loss in red (c).
position process, a threshold value of 30 lm was defined. This means that all areas of the recall replica which differed from the baseline replica by more than 30 lm in the negative direction were not included in the matching process. Matching was accepted when the standard deviations between the image points of the two occlusal surfaces were